# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2017

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_sad1
_database_code_depnum_ccdc_archive 'CCDC 1556452'
_audit_update_record             
;
2017-06-16 deposited with the CCDC.
2017-08-28 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/7
_shelx_SHELXL_version_number     2014/7
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'F8 Fe2 Li5 O4 P'
_chemical_formula_weight         393.37

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      orthorhombic
_space_group_IT_number           54
_space_group_name_H-M_alt        'P c c a'
_space_group_name_Hall           '-P 2a 2ac'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z'
'-x, y, -z+1/2'
'x+1/2, -y, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z'
'x, -y, z-1/2'
'-x-1/2, y, z-1/2'

_cell_length_a                   18.835(11)
_cell_length_b                   9.183(5)
_cell_length_c                   9.479(5)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     1639.7(16)
_cell_formula_units_Z            8
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    1009
_cell_measurement_theta_min      3.27
_cell_measurement_theta_max      28.30

_exptl_crystal_description       diamond
_exptl_crystal_colour            colorless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    3.187
_exptl_crystal_F_000             1488
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.120
_exptl_crystal_size_mid          0.116
_exptl_crystal_size_min          0.030
_exptl_absorpt_coefficient_mu    3.876
_shelx_estimated_absorpt_T_min   0.653
_shelx_estimated_absorpt_T_max   0.893
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.6534
_exptl_absorpt_correction_T_max  0.8926
_exptl_absorpt_process_details   '(SADABS; Bruker, 2008)'
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker Smart-Apex CCD area detector'
_diffrn_measurement_method       'ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            18813
_diffrn_reflns_av_unetI/netI     0.0212
_diffrn_reflns_av_R_equivalents  0.0405
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_theta_min         2.163
_diffrn_reflns_theta_max         28.299
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measured_fraction_theta_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_point_group_measured_fraction_full 1.000
_reflns_number_total             2048
_reflns_number_gt                1856
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker SMART V5.631 (Bruker, 2002)'
_computing_cell_refinement       'Bruker SAINT V7.60A (Bruker, 2008)'
_computing_data_reduction        'Bruker SAINT V7.60A (Bruker, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics    'SHELXTL (Sheldrick, 2008)'
_computing_publication_material  'SHELXTL (Sheldrick, 2008)'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0312P)²+1.5807P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    none
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         2048
_refine_ls_number_parameters     186
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0296
_refine_ls_R_factor_gt           0.0260
_refine_ls_wR_factor_ref         0.0760
_refine_ls_wR_factor_gt          0.0737
_refine_ls_goodness_of_fit_ref   1.205
_refine_ls_restrained_S_all      1.205
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Fe1 Fe 0.37601(2) 0.51532(4) 0.27215(4) 0.00829(11) Uani 1 1 d . . . . .
Fe2 Fe 0.2500 1.0000 -0.04605(5) 0.00869(13) Uani 1 2 d S T P . .
Fe3 Fe 0.5000 1.0000 0.0000 0.00833(13) Uani 1 2 d S . P . .
P1 P 0.37435(3) 0.74656(7) 0.00677(6) 0.00708(14) Uani 1 1 d . . . . .
O1 O 0.31682(9) 0.83157(18) -0.07309(17) 0.0120(3) Uani 1 1 d . . . . .
O2 O 0.33937(8) 0.65843(17) 0.12638(17) 0.0104(3) Uani 1 1 d . . . . .
O3 O 0.42926(8) 0.85150(18) 0.07129(17) 0.0100(3) Uani 1 1 d . . . . .
O4 O 0.41226(8) 0.64232(18) -0.09649(17) 0.0094(3) Uani 1 1 d . . . . .
F1 F 0.44384(7) 0.64609(15) 0.35583(15) 0.0140(3) Uani 1 1 d . . . . .
F2 F 0.44287(7) 0.43440(16) 0.14193(14) 0.0136(3) Uani 1 1 d . . . . .
F3 F 0.54925(7) 0.85730(15) -0.12015(15) 0.0131(3) Uani 1 1 d . . . . .
F4 F 0.30643(7) 0.38820(15) 0.19217(15) 0.0143(3) Uani 1 1 d . . . . .
F5 F 0.30977(7) 0.59885(15) 0.40567(15) 0.0141(3) Uani 1 1 d . . . . .
F6 F 0.55805(7) 0.94338(16) 0.15107(14) 0.0143(3) Uani 1 1 d . . . . .
F7 F 0.30736(7) 1.10281(15) 0.09011(15) 0.0158(3) Uani 1 1 d . . . . .
F8 F 0.30515(7) 1.09828(15) -0.18947(15) 0.0145(3) Uani 1 1 d . . . . .
Li1 Li 0.2500 0.5000 0.5506(7) 0.0201(14) Uani 1 2 d S T P . .
Li2 Li 0.5000 0.5000 0.0000 0.0291(18) Uani 1 2 d S . P . .
Li3 Li 0.6239(2) 1.0111(6) 0.2834(5) 0.0218(11) Uani 1 1 d . . . . .
Li4 Li 0.5000 0.7893(7) 0.2500 0.0181(13) Uani 1 2 d S T P . .
Li5 Li 0.5000 0.7160(8) -0.2500 0.0231(15) Uani 1 2 d S T P . .
Li6 Li 0.2460(3) 0.2546(7) 0.2584(7) 0.0367(15) Uani 1 1 d . . . . .
Li7 Li 0.3765(3) 0.7436(9) 0.5112(9) 0.060(3) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Fe1 F4 1.9118(16) . ?
Fe1 F2 1.9136(15) . ?
Fe1 F1 1.9246(15) . ?
Fe1 F5 1.9357(15) . ?
Fe1 O4 2.0279(18) 7_566 ?
Fe1 O2 2.0281(18) . ?
Fe1 Li7 3.087(6) . ?
Fe1 Li6 3.124(6) 2_565 ?
Fe1 Li5 3.164(5) 5_665 ?
Fe1 Li1 3.172(5) 7_565 ?
Fe1 Li2 3.1842(13) 3_655 ?
Fe2 F7 1.9300(16) . ?
Fe2 F7 1.9300(16) 2_575 ?
Fe2 F8 1.9344(16) 2_575 ?
Fe2 F8 1.9344(16) . ?
Fe2 O1 2.0105(18) 2_575 ?
Fe2 O1 2.0105(18) . ?
Fe2 Li6 2.985(6) 7_565 ?
Fe2 Li6 2.985(6) 8_665 ?
Fe3 F6 1.8753(15) . ?
Fe3 F6 1.8753(15) 5_675 ?
Fe3 F3 1.9685(15) 5_675 ?
Fe3 F3 1.9685(15) . ?
Fe3 O3 2.0229(18) . ?
Fe3 O3 2.0229(18) 5_675 ?
Fe3 Li4 3.060(4) 5_675 ?
Fe3 Li4 3.060(4) . ?
Fe3 Li3 3.109(5) 3_655 ?
Fe3 Li3 3.109(5) 7_575 ?
P1 O1 1.5352(18) . ?
P1 O3 1.5402(18) . ?
P1 O2 1.5411(17) . ?
P1 O4 1.5441(17) . ?
O1 Li6 2.227(6) 7_565 ?
O2 Li6 2.188(6) 2_565 ?
O2 Li1 2.338(3) 7_565 ?
O3 Li4 2.230(2) . ?
O3 Li3 2.246(6) 3_655 ?
O4 Fe1 2.0280(18) 7_565 ?
O4 Li2 2.2969(18) . ?
O4 Li5 2.304(3) . ?
F1 Li4 1.963(5) . ?
F1 Li7 2.140(7) . ?
F1 Li2 2.1878(16) 3_655 ?
F2 Li2 1.8251(15) . ?
F2 Li5 2.029(5) 5_665 ?
F2 Li7 2.402(9) 7_565 ?
F3 Li5 2.015(5) . ?
F3 Li7 2.028(6) 3_655 ?
F3 Li3 2.067(5) 7_575 ?
F4 Li6 1.787(5) . ?
F4 Li1 1.996(5) 7_565 ?
F4 Li7 2.480(9) 7_565 ?
F5 Li1 1.995(5) . ?
F5 Li7 2.085(6) . ?
F5 Li6 2.205(8) 2_565 ?
F6 Li3 1.870(5) . ?
F6 Li4 2.019(5) . ?
F7 Li3 1.956(5) 3_655 ?
F7 Li7 2.061(6) 7_575 ?
F7 Li6 2.413(8) 1_565 ?
F8 Li6 1.798(5) 8_665 ?
F8 Li3 1.895(5) 5_675 ?
Li1 F5 1.995(5) 2_565 ?
Li1 F4 1.996(5) 7_566 ?
Li1 F4 1.996(5) 8_656 ?
Li1 O2 2.338(3) 7_566 ?
Li1 O2 2.338(3) 8_656 ?
Li1 Li6 2.994(7) 7_566 ?
Li1 Li6 2.994(7) 8_656 ?
Li1 Fe1 3.172(5) 7_566 ?
Li1 Fe1 3.172(5) 8_656 ?
Li1 Li7 3.289(8) . ?
Li1 Li7 3.289(8) 2_565 ?
Li2 F2 1.8251(15) 5_665 ?
Li2 F1 2.1878(16) 7_565 ?
Li2 F1 2.1878(16) 3_655 ?
Li2 O4 2.2969(18) 5_665 ?
Li2 Li5 3.091(5) 5_665 ?
Li2 Li5 3.091(5) . ?
Li2 Fe1 3.1842(13) 3_655 ?
Li2 Fe1 3.1842(13) 7_565 ?
Li2 Li7 3.229(7) 7_565 ?
Li2 Li7 3.229(7) 3_655 ?
Li3 F8 1.895(5) 5_675 ?
Li3 F7 1.956(5) 3_655 ?
Li3 F3 2.067(5) 7_576 ?
Li3 O3 2.246(6) 3_655 ?
Li3 Li7 2.978(8) 5_676 ?
Li3 Fe3 3.109(5) 3_655 ?
Li3 Li4 3.113(7) . ?
Li3 Li6 3.342(8) 3_665 ?
Li3 Li6 3.377(7) 4_565 ?
Li3 Li5 3.438(7) 5_675 ?
Li4 F1 1.963(5) 3_655 ?
Li4 F6 2.019(5) 3_655 ?
Li4 O3 2.230(2) 3_655 ?
Li4 Fe3 3.060(4) 3_655 ?
Li4 Li3 3.113(6) 3_655 ?
Li4 Li7 3.423(8) 3_655 ?
Li4 Li7 3.423(8) . ?
Li5 F3 2.015(5) 3_654 ?
Li5 F2 2.029(5) 7_565 ?
Li5 F2 2.029(5) 5_665 ?
Li5 O4 2.304(3) 3_654 ?
Li5 Li2 3.091(5) 3_654 ?
Li5 Fe1 3.164(5) 7_565 ?
Li5 Fe1 3.164(5) 5_665 ?
Li5 Li7 3.255(8) 3_655 ?
Li5 Li7 3.255(8) 1_554 ?
Li6 F8 1.798(5) 8_646 ?
Li6 O2 2.188(6) 2_565 ?
Li6 F5 2.205(8) 2_565 ?
Li6 O1 2.227(6) 7_566 ?
Li6 F7 2.413(8) 1_545 ?
Li6 Fe2 2.985(6) 7_566 ?
Li6 Li1 2.994(7) 7_565 ?
Li6 Fe1 3.124(6) 2_565 ?
Li6 Li7 3.327(10) 2_565 ?
Li6 Li3 3.342(8) 3_645 ?
Li6 Li3 3.377(7) 4_465 ?
Li7 F3 2.028(6) 3_655 ?
Li7 F7 2.061(6) 7_576 ?
Li7 F2 2.402(9) 7_566 ?
Li7 F4 2.480(9) 7_566 ?
Li7 Li3 2.978(8) 5_676 ?
Li7 Li2 3.229(7) 3_655 ?
Li7 Li5 3.255(8) 1_556 ?
Li7 Li6 3.327(10) 2_565 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F4 Fe1 F2 87.60(7) . . ?
F4 Fe1 F1 178.29(6) . . ?
F2 Fe1 F1 94.08(7) . . ?
F4 Fe1 F5 93.41(7) . . ?
F2 Fe1 F5 178.96(6) . . ?
F1 Fe1 F5 84.90(7) . . ?
F4 Fe1 O4 92.20(7) . 7_566 ?
F2 Fe1 O4 84.11(7) . 7_566 ?
F1 Fe1 O4 88.21(7) . 7_566 ?
F5 Fe1 O4 95.65(7) . 7_566 ?
F4 Fe1 O2 83.81(7) . . ?
F2 Fe1 O2 92.07(7) . . ?
F1 Fe1 O2 95.87(7) . . ?
F5 Fe1 O2 88.25(7) . . ?
O4 Fe1 O2 174.60(7) 7_566 . ?
F4 Fe1 Li7 135.06(12) . . ?
F2 Fe1 Li7 137.32(12) . . ?
F1 Fe1 Li7 43.25(12) . . ?
F5 Fe1 Li7 41.66(12) . . ?
O4 Fe1 Li7 91.88(19) 7_566 . ?
O2 Fe1 Li7 93.51(19) . . ?
F4 Fe1 Li6 83.81(11) . 2_565 ?
F2 Fe1 Li6 136.03(14) . 2_565 ?
F1 Fe1 Li6 94.79(11) . 2_565 ?
F5 Fe1 Li6 44.38(14) . 2_565 ?
O4 Fe1 Li6 139.11(14) 7_566 2_565 ?
O2 Fe1 Li6 44.19(14) . 2_565 ?
Li7 Fe1 Li6 64.78(18) . 2_565 ?
F4 Fe1 Li5 93.99(10) . 5_665 ?
F2 Fe1 Li5 37.88(5) . 5_665 ?
F1 Fe1 Li5 87.50(10) . 5_665 ?
F5 Fe1 Li5 141.74(5) . 5_665 ?
O4 Fe1 Li5 46.60(7) 7_566 5_665 ?
O2 Fe1 Li5 129.87(6) . 5_665 ?
Li7 Fe1 Li5 120.15(14) . 5_665 ?
Li6 Fe1 Li5 173.79(13) 2_565 5_665 ?
F4 Fe1 Li1 36.63(5) . 7_565 ?
F2 Fe1 Li1 92.76(10) . 7_565 ?
F1 Fe1 Li1 142.87(5) . 7_565 ?
F5 Fe1 Li1 88.18(10) . 7_565 ?
O4 Fe1 Li1 128.81(6) 7_566 7_565 ?
O2 Fe1 Li1 47.39(6) . 7_565 ?
Li7 Fe1 Li1 121.23(14) . 7_565 ?
Li6 Fe1 Li1 56.77(12) 2_565 7_565 ?
Li5 Fe1 Li1 118.59(8) 5_665 7_565 ?
F4 Fe1 Li2 138.14(5) . 3_655 ?
F2 Fe1 Li2 86.43(6) . 3_655 ?
F1 Fe1 Li2 42.36(5) . 3_655 ?
F5 Fe1 Li2 92.68(6) . 3_655 ?
O4 Fe1 Li2 45.97(5) 7_566 3_655 ?
O2 Fe1 Li2 137.76(5) . 3_655 ?
Li7 Fe1 Li2 61.95(14) . 3_655 ?
Li6 Fe1 Li2 126.70(11) 2_565 3_655 ?
Li5 Fe1 Li2 58.27(5) 5_665 3_655 ?
Li1 Fe1 Li2 174.77(3) 7_565 3_655 ?
F7 Fe2 F7 96.05(10) . 2_575 ?
F7 Fe2 F8 177.32(7) . 2_575 ?
F7 Fe2 F8 86.63(7) 2_575 2_575 ?
F7 Fe2 F8 86.63(7) . . ?
F7 Fe2 F8 177.31(7) 2_575 . ?
F8 Fe2 F8 90.69(10) 2_575 . ?
F7 Fe2 O1 93.40(7) . 2_575 ?
F7 Fe2 O1 96.38(7) 2_575 2_575 ?
F8 Fe2 O1 86.17(7) 2_575 2_575 ?
F8 Fe2 O1 83.55(7) . 2_575 ?
F7 Fe2 O1 96.38(7) . . ?
F7 Fe2 O1 93.40(7) 2_575 . ?
F8 Fe2 O1 83.54(7) 2_575 . ?
F8 Fe2 O1 86.17(7) . . ?
O1 Fe2 O1 165.35(10) 2_575 . ?
F7 Fe2 Li6 144.36(11) . 7_565 ?
F7 Fe2 Li6 91.03(15) 2_575 7_565 ?
F8 Fe2 Li6 35.36(11) 2_575 7_565 ?
F8 Fe2 Li6 86.71(15) . 7_565 ?
O1 Fe2 Li6 120.51(13) 2_575 7_565 ?
O1 Fe2 Li6 48.24(11) . 7_565 ?
F7 Fe2 Li6 91.03(15) . 8_665 ?
F7 Fe2 Li6 144.36(11) 2_575 8_665 ?
F8 Fe2 Li6 86.71(15) 2_575 8_665 ?
F8 Fe2 Li6 35.36(11) . 8_665 ?
O1 Fe2 Li6 48.24(12) 2_575 8_665 ?
O1 Fe2 Li6 120.51(13) . 8_665 ?
Li6 Fe2 Li6 103.2(3) 7_565 8_665 ?
F6 Fe3 F6 180.0 . 5_675 ?
F6 Fe3 F3 91.00(7) . 5_675 ?
F6 Fe3 F3 89.00(7) 5_675 5_675 ?
F6 Fe3 F3 89.00(7) . . ?
F6 Fe3 F3 91.00(7) 5_675 . ?
F3 Fe3 F3 180.00(7) 5_675 . ?
F6 Fe3 O3 86.68(7) . . ?
F6 Fe3 O3 93.32(7) 5_675 . ?
F3 Fe3 O3 86.85(7) 5_675 . ?
F3 Fe3 O3 93.15(7) . . ?
F6 Fe3 O3 93.32(7) . 5_675 ?
F6 Fe3 O3 86.68(7) 5_675 5_675 ?
F3 Fe3 O3 93.15(7) 5_675 5_675 ?
F3 Fe3 O3 86.85(7) . 5_675 ?
O3 Fe3 O3 180.0 . 5_675 ?
F6 Fe3 Li4 140.07(6) . 5_675 ?
F6 Fe3 Li4 39.93(6) 5_675 5_675 ?
F3 Fe3 Li4 91.55(10) 5_675 5_675 ?
F3 Fe3 Li4 88.45(10) . 5_675 ?
O3 Fe3 Li4 133.25(6) . 5_675 ?
O3 Fe3 Li4 46.75(6) 5_675 5_675 ?
F6 Fe3 Li4 39.93(6) . . ?
F6 Fe3 Li4 140.07(6) 5_675 . ?
F3 Fe3 Li4 88.45(10) 5_675 . ?
F3 Fe3 Li4 91.55(10) . . ?
O3 Fe3 Li4 46.75(6) . . ?
O3 Fe3 Li4 133.25(6) 5_675 . ?
Li4 Fe3 Li4 180.0 5_675 . ?
F6 Fe3 Li3 86.69(10) . 3_655 ?
F6 Fe3 Li3 93.31(10) 5_675 3_655 ?
F3 Fe3 Li3 40.77(11) 5_675 3_655 ?
F3 Fe3 Li3 139.24(11) . 3_655 ?
O3 Fe3 Li3 46.15(11) . 3_655 ?
O3 Fe3 Li3 133.85(11) 5_675 3_655 ?
Li4 Fe3 Li3 119.39(10) 5_675 3_655 ?
Li4 Fe3 Li3 60.61(10) . 3_655 ?
F6 Fe3 Li3 93.31(10) . 7_575 ?
F6 Fe3 Li3 86.69(10) 5_675 7_575 ?
F3 Fe3 Li3 139.23(11) 5_675 7_575 ?
F3 Fe3 Li3 40.76(11) . 7_575 ?
O3 Fe3 Li3 133.85(11) . 7_575 ?
O3 Fe3 Li3 46.15(11) 5_675 7_575 ?
Li4 Fe3 Li3 60.61(10) 5_675 7_575 ?
Li4 Fe3 Li3 119.39(10) . 7_575 ?
Li3 Fe3 Li3 180.0 3_655 7_575 ?
O1 P1 O3 110.58(10) . . ?
O1 P1 O2 109.15(10) . . ?
O3 P1 O2 108.87(10) . . ?
O1 P1 O4 109.22(10) . . ?
O3 P1 O4 109.22(10) . . ?
O2 P1 O4 109.79(10) . . ?
P1 O1 Fe2 140.38(11) . . ?
P1 O1 Li6 126.57(17) . 7_565 ?
Fe2 O1 Li6 89.43(15) . 7_565 ?
P1 O2 Fe1 134.12(10) . . ?
P1 O2 Li6 122.9(2) . 2_565 ?
Fe1 O2 Li6 95.6(2) . 2_565 ?
P1 O2 Li1 114.12(18) . 7_565 ?
Fe1 O2 Li1 92.93(13) . 7_565 ?
Li6 O2 Li1 82.75(18) 2_565 7_565 ?
P1 O3 Fe3 137.00(10) . . ?
P1 O3 Li4 122.86(18) . . ?
Fe3 O3 Li4 91.89(13) . . ?
P1 O3 Li3 110.66(15) . 3_655 ?
Fe3 O3 Li3 93.35(14) . 3_655 ?
Li4 O3 Li3 88.14(17) . 3_655 ?
P1 O4 Fe1 132.54(10) . 7_565 ?
P1 O4 Li2 115.66(9) . . ?
Fe1 O4 Li2 94.62(7) 7_565 . ?
P1 O4 Li5 123.36(19) . . ?
Fe1 O4 Li5 93.64(14) 7_565 . ?
Li2 O4 Li5 84.41(12) . . ?
Fe1 F1 Li4 124.40(10) . . ?
Fe1 F1 Li7 98.70(17) . . ?
Li4 F1 Li7 113.0(3) . . ?
Fe1 F1 Li2 101.29(7) . 3_655 ?
Li4 F1 Li2 118.00(10) . 3_655 ?
Li7 F1 Li2 96.5(3) . 3_655 ?
Li2 F2 Fe1 137.34(9) . . ?
Li2 F2 Li5 106.52(8) . 5_665 ?
Fe1 F2 Li5 106.72(8) . 5_665 ?
Li2 F2 Li7 98.69(19) . 7_565 ?
Fe1 F2 Li7 104.74(19) . 7_565 ?
Li5 F2 Li7 94.2(2) 5_665 7_565 ?
Fe3 F3 Li5 124.42(11) . . ?
Fe3 F3 Li7 111.9(3) . 3_655 ?
Li5 F3 Li7 107.3(3) . 3_655 ?
Fe3 F3 Li3 100.78(16) . 7_575 ?
Li5 F3 Li3 114.79(18) . 7_575 ?
Li7 F3 Li3 93.3(2) 3_655 7_575 ?
Li6 F4 Fe1 135.8(2) . . ?
Li6 F4 Li1 104.48(19) . 7_565 ?
Fe1 F4 Li1 108.51(8) . 7_565 ?
Li6 F4 Li7 104.3(3) . 7_565 ?
Fe1 F4 Li7 101.97(18) . 7_565 ?
Li1 F4 Li7 94.0(2) 7_565 7_565 ?
Fe1 F5 Li1 129.33(10) . . ?
Fe1 F5 Li7 100.24(19) . . ?
Li1 F5 Li7 107.4(3) . . ?
Fe1 F5 Li6 97.75(16) . 2_565 ?
Li1 F5 Li6 116.42(17) . 2_565 ?
Li7 F5 Li6 101.7(3) . 2_565 ?
Li3 F6 Fe3 143.77(18) . . ?
Li3 F6 Li4 106.28(18) . . ?
Fe3 F6 Li4 103.49(7) . . ?
Fe2 F7 Li3 124.76(17) . 3_655 ?
Fe2 F7 Li7 116.5(3) . 7_575 ?
Li3 F7 Li7 95.7(2) 3_655 7_575 ?
Fe2 F7 Li6 117.17(15) . 1_565 ?
Li3 F7 Li6 99.3(2) 3_655 1_565 ?
Li7 F7 Li6 98.5(3) 7_575 1_565 ?
Li6 F8 Li3 132.2(3) 8_665 5_675 ?
Li6 F8 Fe2 106.14(19) 8_665 . ?
Li3 F8 Fe2 117.52(18) 5_675 . ?
F5 Li1 F5 92.9(3) 2_565 . ?
F5 Li1 F4 176.03(11) 2_565 7_566 ?
F5 Li1 F4 85.90(7) . 7_566 ?
F5 Li1 F4 85.90(7) 2_565 8_656 ?
F5 Li1 F4 176.03(11) . 8_656 ?
F4 Li1 F4 95.5(3) 7_566 8_656 ?
F5 Li1 O2 109.55(11) 2_565 7_566 ?
F5 Li1 O2 95.08(9) . 7_566 ?
F4 Li1 O2 74.35(14) 7_566 7_566 ?
F4 Li1 O2 81.76(16) 8_656 7_566 ?
F5 Li1 O2 95.08(9) 2_565 8_656 ?
F5 Li1 O2 109.56(11) . 8_656 ?
F4 Li1 O2 81.76(16) 7_566 8_656 ?
F4 Li1 O2 74.35(14) 8_656 8_656 ?
O2 Li1 O2 144.2(3) 7_566 8_656 ?
F5 Li1 Li6 141.40(11) 2_565 7_566 ?
F5 Li1 Li6 97.17(15) . 7_566 ?
F4 Li1 Li6 35.31(13) 7_566 7_566 ?
F4 Li1 Li6 86.1(3) 8_656 7_566 ?
O2 Li1 Li6 106.5(2) 7_566 7_566 ?
O2 Li1 Li6 46.48(13) 8_656 7_566 ?
F5 Li1 Li6 97.17(15) 2_565 8_656 ?
F5 Li1 Li6 141.39(11) . 8_656 ?
F4 Li1 Li6 86.1(2) 7_566 8_656 ?
F4 Li1 Li6 35.31(13) 8_656 8_656 ?
O2 Li1 Li6 46.48(13) 7_566 8_656 ?
O2 Li1 Li6 106.5(2) 8_656 8_656 ?
Li6 Li1 Li6 97.7(4) 7_566 8_656 ?
F5 Li1 Fe1 149.10(4) 2_565 7_566 ?
F5 Li1 Fe1 93.09(7) . 7_566 ?
F4 Li1 Fe1 34.85(8) 7_566 7_566 ?
F4 Li1 Fe1 86.0(2) 8_656 7_566 ?
O2 Li1 Fe1 39.68(8) 7_566 7_566 ?
O2 Li1 Fe1 111.3(2) 8_656 7_566 ?
Li6 Li1 Fe1 67.46(16) 7_566 7_566 ?
Li6 Li1 Fe1 60.81(16) 8_656 7_566 ?
F5 Li1 Fe1 93.09(7) 2_565 8_656 ?
F5 Li1 Fe1 149.10(4) . 8_656 ?
F4 Li1 Fe1 86.0(2) 7_566 8_656 ?
F4 Li1 Fe1 34.85(8) 8_656 8_656 ?
O2 Li1 Fe1 111.3(2) 7_566 8_656 ?
O2 Li1 Fe1 39.68(8) 8_656 8_656 ?
Li6 Li1 Fe1 60.81(16) 7_566 8_656 ?
Li6 Li1 Fe1 67.46(16) 8_656 8_656 ?
Fe1 Li1 Fe1 97.09(19) 7_566 8_656 ?
F5 Li1 Li7 129.8(3) 2_565 . ?
F5 Li1 Li7 37.21(15) . . ?
F4 Li1 Li7 48.76(16) 7_566 . ?
F4 Li1 Li7 144.3(3) 8_656 . ?
O2 Li1 Li7 86.36(16) 7_566 . ?
O2 Li1 Li7 97.66(13) 8_656 . ?
Li6 Li1 Li7 65.23(18) 7_566 . ?
Li6 Li1 Li7 124.6(2) 8_656 . ?
Fe1 Li1 Li7 64.10(17) 7_566 . ?
Fe1 Li1 Li7 125.94(17) 8_656 . ?
F5 Li1 Li7 37.21(15) 2_565 2_565 ?
F5 Li1 Li7 129.8(3) . 2_565 ?
F4 Li1 Li7 144.3(3) 7_566 2_565 ?
F4 Li1 Li7 48.76(16) 8_656 2_565 ?
O2 Li1 Li7 97.66(13) 7_566 2_565 ?
O2 Li1 Li7 86.36(16) 8_656 2_565 ?
Li6 Li1 Li7 124.6(2) 7_566 2_565 ?
Li6 Li1 Li7 65.23(18) 8_656 2_565 ?
Fe1 Li1 Li7 125.94(17) 7_566 2_565 ?
Fe1 Li1 Li7 64.10(17) 8_656 2_565 ?
Li7 Li1 Li7 167.0(4) . 2_565 ?
F2 Li2 F2 180.0 . 5_665 ?
F2 Li2 F1 88.46(7) . 7_565 ?
F2 Li2 F1 91.54(7) 5_665 7_565 ?
F2 Li2 F1 91.54(7) . 3_655 ?
F2 Li2 F1 88.46(7) 5_665 3_655 ?
F1 Li2 F1 180.00(8) 7_565 3_655 ?
F2 Li2 O4 93.28(7) . . ?
F2 Li2 O4 86.72(7) 5_665 . ?
F1 Li2 O4 75.66(6) 7_565 . ?
F1 Li2 O4 104.34(6) 3_655 . ?
F2 Li2 O4 86.72(7) . 5_665 ?
F2 Li2 O4 93.28(7) 5_665 5_665 ?
F1 Li2 O4 104.34(6) 7_565 5_665 ?
F1 Li2 O4 75.66(6) 3_655 5_665 ?
O4 Li2 O4 180.0 . 5_665 ?
F2 Li2 Li5 39.00(6) . 5_665 ?
F2 Li2 Li5 141.00(6) 5_665 5_665 ?
F1 Li2 Li5 94.90(10) 7_565 5_665 ?
F1 Li2 Li5 85.10(10) 3_655 5_665 ?
O4 Li2 Li5 132.11(5) . 5_665 ?
O4 Li2 Li5 47.89(5) 5_665 5_665 ?
F2 Li2 Li5 141.00(6) . . ?
F2 Li2 Li5 39.00(6) 5_665 . ?
F1 Li2 Li5 85.10(10) 7_565 . ?
F1 Li2 Li5 94.90(10) 3_655 . ?
O4 Li2 Li5 47.89(5) . . ?
O4 Li2 Li5 132.11(5) 5_665 . ?
Li5 Li2 Li5 180.0 5_665 . ?
F2 Li2 Fe1 86.96(6) . 3_655 ?
F2 Li2 Fe1 93.04(6) 5_665 3_655 ?
F1 Li2 Fe1 143.65(4) 7_565 3_655 ?
F1 Li2 Fe1 36.35(4) 3_655 3_655 ?
O4 Li2 Fe1 140.59(4) . 3_655 ?
O4 Li2 Fe1 39.41(5) 5_665 3_655 ?
Li5 Li2 Fe1 60.54(6) 5_665 3_655 ?
Li5 Li2 Fe1 119.46(6) . 3_655 ?
F2 Li2 Fe1 93.04(6) . 7_565 ?
F2 Li2 Fe1 86.96(6) 5_665 7_565 ?
F1 Li2 Fe1 36.35(4) 7_565 7_565 ?
F1 Li2 Fe1 143.65(4) 3_655 7_565 ?
O4 Li2 Fe1 39.41(4) . 7_565 ?
O4 Li2 Fe1 140.59(5) 5_665 7_565 ?
Li5 Li2 Fe1 119.46(6) 5_665 7_565 ?
Li5 Li2 Fe1 60.54(6) . 7_565 ?
Fe1 Li2 Fe1 180.0 3_655 7_565 ?
F2 Li2 Li7 47.34(17) . 7_565 ?
F2 Li2 Li7 132.66(17) 5_665 7_565 ?
F1 Li2 Li7 41.19(17) 7_565 7_565 ?
F1 Li2 Li7 138.81(17) 3_655 7_565 ?
O4 Li2 Li7 83.63(12) . 7_565 ?
O4 Li2 Li7 96.37(12) 5_665 7_565 ?
Li5 Li2 Li7 61.96(13) 5_665 7_565 ?
Li5 Li2 Li7 118.04(13) . 7_565 ?
Fe1 Li2 Li7 122.45(12) 3_655 7_565 ?
Fe1 Li2 Li7 57.55(12) 7_565 7_565 ?
F2 Li2 Li7 132.66(17) . 3_655 ?
F2 Li2 Li7 47.34(17) 5_665 3_655 ?
F1 Li2 Li7 138.81(17) 7_565 3_655 ?
F1 Li2 Li7 41.19(17) 3_655 3_655 ?
O4 Li2 Li7 96.37(12) . 3_655 ?
O4 Li2 Li7 83.63(12) 5_665 3_655 ?
Li5 Li2 Li7 118.04(13) 5_665 3_655 ?
Li5 Li2 Li7 61.96(13) . 3_655 ?
Fe1 Li2 Li7 57.55(12) 3_655 3_655 ?
Fe1 Li2 Li7 122.45(12) 7_565 3_655 ?
Li7 Li2 Li7 180.0(2) 7_565 3_655 ?
F6 Li3 F8 88.6(2) . 5_675 ?
F6 Li3 F7 173.5(3) . 3_655 ?
F8 Li3 F7 92.8(2) 5_675 3_655 ?
F6 Li3 F3 92.33(19) . 7_576 ?
F8 Li3 F3 176.2(3) 5_675 7_576 ?
F7 Li3 F3 85.8(2) 3_655 7_576 ?
F6 Li3 O3 84.2(2) . 3_655 ?
F8 Li3 O3 104.9(2) 5_675 3_655 ?
F7 Li3 O3 101.5(2) 3_655 3_655 ?
F3 Li3 O3 78.90(18) 7_576 3_655 ?
F6 Li3 Li7 133.5(2) . 5_676 ?
F8 Li3 Li7 135.2(2) 5_675 5_676 ?
F7 Li3 Li7 43.52(16) 3_655 5_676 ?
F3 Li3 Li7 42.83(15) 7_576 5_676 ?
O3 Li3 Li7 95.3(3) 3_655 5_676 ?
F6 Li3 Fe3 86.27(17) . 3_655 ?
F8 Li3 Fe3 145.3(3) 5_675 3_655 ?
F7 Li3 Fe3 96.10(19) 3_655 3_655 ?
F3 Li3 Fe3 38.46(10) 7_576 3_655 ?
O3 Li3 Fe3 40.50(9) 3_655 3_655 ?
Li7 Li3 Fe3 65.88(18) 5_676 3_655 ?
F6 Li3 Li4 38.51(12) . . ?
F8 Li3 Li4 97.7(2) 5_675 . ?
F7 Li3 Li4 147.2(2) 3_655 . ?
F3 Li3 Li4 85.31(17) 7_576 . ?
O3 Li3 Li4 45.72(10) 3_655 . ?
Li7 Li3 Li4 124.0(2) 5_676 . ?
Fe3 Li3 Li4 58.91(10) 3_655 . ?
F6 Li3 Li6 129.0(3) . 3_665 ?
F8 Li3 Li6 77.37(18) 5_675 3_665 ?
F7 Li3 Li6 45.46(17) 3_655 3_665 ?
F3 Li3 Li6 99.2(2) 7_576 3_665 ?
O3 Li3 Li6 146.7(2) 3_655 3_665 ?
Li7 Li3 Li6 64.7(2) 5_676 3_665 ?
Fe3 Li3 Li6 130.58(19) 3_655 3_665 ?
Li4 Li3 Li6 167.3(2) . 3_665 ?
F6 Li3 Li6 97.6(2) . 4_565 ?
F8 Li3 Li6 23.22(14) 5_675 4_565 ?
F7 Li3 Li6 86.1(2) 3_655 4_565 ?
F3 Li3 Li6 159.7(3) 7_576 4_565 ?
O3 Li3 Li6 84.48(18) 3_655 4_565 ?
Li7 Li3 Li6 128.7(2) 5_676 4_565 ?
Fe3 Li3 Li6 124.40(19) 3_655 4_565 ?
Li4 Li3 Li6 91.48(19) . 4_565 ?
Li6 Li3 Li6 88.28(18) 3_665 4_565 ?
F6 Li3 Li5 74.38(16) . 5_675 ?
F8 Li3 Li5 145.3(2) 5_675 5_675 ?
F7 Li3 Li5 101.1(2) 3_655 5_675 ?
F3 Li3 Li5 32.13(9) 7_576 5_675 ?
O3 Li3 Li5 103.29(17) 3_655 5_675 ?
Li7 Li3 Li5 60.47(18) 5_676 5_675 ?
Fe3 Li3 Li5 64.89(10) 3_655 5_675 ?
Li4 Li3 Li5 87.66(16) . 5_675 ?
Li6 Li3 Li5 89.94(18) 3_665 5_675 ?
Li6 Li3 Li5 168.0(2) 4_565 5_675 ?
F1 Li4 F1 95.9(3) 3_655 . ?
F1 Li4 F6 176.8(2) 3_655 3_655 ?
F1 Li4 F6 86.58(7) . 3_655 ?
F1 Li4 F6 86.58(7) 3_655 . ?
F1 Li4 F6 176.8(2) . . ?
F6 Li4 F6 91.0(3) 3_655 . ?
F1 Li4 O3 96.05(10) 3_655 . ?
F1 Li4 O3 103.76(11) . . ?
F6 Li4 O3 81.35(16) 3_655 . ?
F6 Li4 O3 77.94(15) . . ?
F1 Li4 O3 103.76(11) 3_655 3_655 ?
F1 Li4 O3 96.05(10) . 3_655 ?
F6 Li4 O3 77.95(15) 3_655 3_655 ?
F6 Li4 O3 81.35(16) . 3_655 ?
O3 Li4 O3 150.3(3) . 3_655 ?
F1 Li4 Fe3 145.03(4) 3_655 3_655 ?
F1 Li4 Fe3 91.60(7) . 3_655 ?
F6 Li4 Fe3 36.59(7) 3_655 3_655 ?
F6 Li4 Fe3 85.21(19) . 3_655 ?
O3 Li4 Fe3 115.2(2) . 3_655 ?
O3 Li4 Fe3 41.36(9) 3_655 3_655 ?
F1 Li4 Fe3 91.60(7) 3_655 . ?
F1 Li4 Fe3 145.03(4) . . ?
F6 Li4 Fe3 85.2(2) 3_655 . ?
F6 Li4 Fe3 36.58(7) . . ?
O3 Li4 Fe3 41.36(9) . . ?
O3 Li4 Fe3 115.2(2) 3_655 . ?
Fe3 Li4 Fe3 101.5(2) 3_655 . ?
F1 Li4 Li3 94.97(11) 3_655 . ?
F1 Li4 Li3 142.18(10) . . ?
F6 Li4 Li3 84.3(2) 3_655 . ?
F6 Li4 Li3 35.21(12) . . ?
O3 Li4 Li3 110.9(2) . . ?
O3 Li4 Li3 46.15(13) 3_655 . ?
Fe3 Li4 Li3 60.48(13) 3_655 . ?
Fe3 Li4 Li3 70.42(15) . . ?
F1 Li4 Li3 142.18(10) 3_655 3_655 ?
F1 Li4 Li3 94.96(11) . 3_655 ?
F6 Li4 Li3 35.21(12) 3_655 3_655 ?
F6 Li4 Li3 84.3(2) . 3_655 ?
O3 Li4 Li3 46.15(13) . 3_655 ?
O3 Li4 Li3 110.9(2) 3_655 3_655 ?
Fe3 Li4 Li3 70.42(15) 3_655 3_655 ?
Fe3 Li4 Li3 60.49(13) . 3_655 ?
Li3 Li4 Li3 98.3(3) . 3_655 ?
F1 Li4 Li7 35.13(14) 3_655 3_655 ?
F1 Li4 Li7 130.8(3) . 3_655 ?
F6 Li4 Li7 142.2(3) 3_655 3_655 ?
F6 Li4 Li7 51.84(15) . 3_655 ?
O3 Li4 Li7 83.56(12) . 3_655 ?
O3 Li4 Li7 100.08(15) 3_655 3_655 ?
Fe3 Li4 Li7 129.6(2) 3_655 3_655 ?
Fe3 Li4 Li7 61.13(11) . 3_655 ?
Li3 Li4 Li7 69.19(19) . 3_655 ?
Li3 Li4 Li7 121.05(17) 3_655 3_655 ?
F1 Li4 Li7 130.8(3) 3_655 . ?
F1 Li4 Li7 35.13(14) . . ?
F6 Li4 Li7 51.84(15) 3_655 . ?
F6 Li4 Li7 142.2(3) . . ?
O3 Li4 Li7 100.08(15) . . ?
O3 Li4 Li7 83.56(12) 3_655 . ?
Fe3 Li4 Li7 61.13(11) 3_655 . ?
Fe3 Li4 Li7 129.6(2) . . ?
Li3 Li4 Li7 121.05(17) . . ?
Li3 Li4 Li7 69.19(19) 3_655 . ?
Li7 Li4 Li7 165.9(4) 3_655 . ?
F3 Li5 F3 99.8(3) 3_654 . ?
F3 Li5 F2 83.44(7) 3_654 7_565 ?
F3 Li5 F2 172.41(12) . 7_565 ?
F3 Li5 F2 172.41(12) 3_654 5_665 ?
F3 Li5 F2 83.44(7) . 5_665 ?
F2 Li5 F2 94.2(3) 7_565 5_665 ?
F3 Li5 O4 97.68(9) 3_654 3_654 ?
F3 Li5 O4 104.18(10) . 3_654 ?
F2 Li5 O4 82.03(16) 7_565 3_654 ?
F2 Li5 O4 74.83(15) 5_665 3_654 ?
F3 Li5 O4 104.18(10) 3_654 . ?
F3 Li5 O4 97.68(9) . . ?
F2 Li5 O4 74.83(15) 7_565 . ?
F2 Li5 O4 82.03(16) 5_665 . ?
O4 Li5 O4 145.8(3) 3_654 . ?
F3 Li5 Li2 86.84(7) 3_654 3_654 ?
F3 Li5 Li2 151.87(4) . 3_654 ?
F2 Li5 Li2 34.48(7) 7_565 3_654 ?
F2 Li5 Li2 87.1(2) 5_665 3_654 ?
O4 Li5 Li2 47.70(9) 3_654 3_654 ?
O4 Li5 Li2 107.2(2) . 3_654 ?
F3 Li5 Li2 151.87(4) 3_654 . ?
F3 Li5 Li2 86.84(7) . . ?
F2 Li5 Li2 87.1(2) 7_565 . ?
F2 Li5 Li2 34.48(7) 5_665 . ?
O4 Li5 Li2 107.2(2) 3_654 . ?
O4 Li5 Li2 47.70(9) . . ?
Li2 Li5 Li2 100.1(2) 3_654 . ?
F3 Li5 Fe1 97.65(7) 3_654 7_565 ?
F3 Li5 Fe1 137.03(5) . 7_565 ?
F2 Li5 Fe1 35.39(8) 7_565 7_565 ?
F2 Li5 Fe1 84.3(2) 5_665 7_565 ?
O4 Li5 Fe1 112.0(2) 3_654 7_565 ?
O4 Li5 Fe1 39.76(9) . 7_565 ?
Li2 Li5 Fe1 67.66(11) 3_654 7_565 ?
Li2 Li5 Fe1 61.19(10) . 7_565 ?
F3 Li5 Fe1 137.03(5) 3_654 5_665 ?
F3 Li5 Fe1 97.65(7) . 5_665 ?
F2 Li5 Fe1 84.3(2) 7_565 5_665 ?
F2 Li5 Fe1 35.39(8) 5_665 5_665 ?
O4 Li5 Fe1 39.76(9) 3_654 5_665 ?
O4 Li5 Fe1 112.0(2) . 5_665 ?
Li2 Li5 Fe1 61.19(10) 3_654 5_665 ?
Li2 Li5 Fe1 67.66(11) . 5_665 ?
Fe1 Li5 Fe1 95.64(19) 7_565 5_665 ?
F3 Li5 Li7 134.7(3) 3_654 3_655 ?
F3 Li5 Li7 36.50(16) . 3_655 ?
F2 Li5 Li7 141.5(3) 7_565 3_655 ?
F2 Li5 Li7 47.38(15) 5_665 3_655 ?
O4 Li5 Li7 87.10(16) 3_654 3_655 ?
O4 Li5 Li7 95.52(13) . 3_655 ?
Li2 Li5 Li7 125.7(2) 3_654 3_655 ?
Li2 Li5 Li7 61.10(12) . 3_655 ?
Fe1 Li5 Li7 122.23(18) 7_565 3_655 ?
Fe1 Li5 Li7 64.59(17) 5_665 3_655 ?
F3 Li5 Li7 36.50(16) 3_654 1_554 ?
F3 Li5 Li7 134.7(3) . 1_554 ?
F2 Li5 Li7 47.38(15) 7_565 1_554 ?
F2 Li5 Li7 141.5(3) 5_665 1_554 ?
O4 Li5 Li7 95.52(13) 3_654 1_554 ?
O4 Li5 Li7 87.10(16) . 1_554 ?
Li2 Li5 Li7 61.10(12) 3_654 1_554 ?
Li2 Li5 Li7 125.7(2) . 1_554 ?
Fe1 Li5 Li7 64.59(17) 7_565 1_554 ?
Fe1 Li5 Li7 122.23(18) 5_665 1_554 ?
Li7 Li5 Li7 171.1(4) 3_655 1_554 ?
F4 Li6 F8 170.3(4) . 8_646 ?
F4 Li6 O2 91.0(2) . 2_565 ?
F8 Li6 O2 93.1(2) 8_646 2_565 ?
F4 Li6 F5 96.1(3) . 2_565 ?
F8 Li6 F5 93.3(3) 8_646 2_565 ?
O2 Li6 F5 77.8(2) 2_565 2_565 ?
F4 Li6 O1 96.6(2) . 7_566 ?
F8 Li6 O1 80.8(2) 8_646 7_566 ?
O2 Li6 O1 168.6(3) 2_565 7_566 ?
F5 Li6 O1 92.8(3) 2_565 7_566 ?
F4 Li6 F7 81.9(2) . 1_545 ?
F8 Li6 F7 88.7(3) 8_646 1_545 ?
O2 Li6 F7 100.6(3) 2_565 1_545 ?
F5 Li6 F7 177.5(3) 2_565 1_545 ?
O1 Li6 F7 89.0(2) 7_566 1_545 ?
F4 Li6 Fe2 137.7(3) . 7_566 ?
F8 Li6 Fe2 38.50(12) 8_646 7_566 ?
O2 Li6 Fe2 131.3(2) 2_565 7_566 ?
F5 Li6 Fe2 95.6(2) 2_565 7_566 ?
O1 Li6 Fe2 42.34(10) 7_566 7_566 ?
F7 Li6 Fe2 86.90(19) 1_545 7_566 ?
F4 Li6 Li1 40.21(13) . 7_565 ?
F8 Li6 Li1 142.7(3) 8_646 7_565 ?
O2 Li6 Li1 50.78(12) 2_565 7_565 ?
F5 Li6 Li1 88.2(2) 2_565 7_565 ?
O1 Li6 Li1 136.4(2) 7_566 7_565 ?
F7 Li6 Li1 89.3(2) 1_545 7_565 ?
Fe2 Li6 Li1 176.0(3) 7_566 7_565 ?
F4 Li6 Fe1 91.1(2) . 2_565 ?
F8 Li6 Fe1 97.7(2) 8_646 2_565 ?
O2 Li6 Fe1 40.25(12) 2_565 2_565 ?
F5 Li6 Fe1 37.87(10) 2_565 2_565 ?
O1 Li6 Fe1 130.6(3) 7_566 2_565 ?
F7 Li6 Fe1 140.4(2) 1_545 2_565 ?
Fe2 Li6 Fe1 121.5(2) 7_566 2_565 ?
Li1 Li6 Fe1 62.42(12) 7_565 2_565 ?
F4 Li6 Li7 133.7(4) . 2_565 ?
F8 Li6 Li7 55.6(2) 8_646 2_565 ?
O2 Li6 Li7 84.3(2) 2_565 2_565 ?
F5 Li6 Li7 37.86(19) 2_565 2_565 ?
O1 Li6 Li7 84.3(2) 7_566 2_565 ?
F7 Li6 Li7 144.2(3) 1_545 2_565 ?
Fe2 Li6 Li7 64.79(17) 7_566 2_565 ?
Li1 Li6 Li7 119.2(3) 7_565 2_565 ?
Fe1 Li6 Li7 57.07(16) 2_565 2_565 ?
F4 Li6 Li3 87.2(2) . 3_645 ?
F8 Li6 Li3 83.8(2) 8_646 3_645 ?
O2 Li6 Li3 135.7(3) 2_565 3_645 ?
F5 Li6 Li3 146.4(3) 2_565 3_645 ?
O1 Li6 Li3 53.68(16) 7_566 3_645 ?
F7 Li6 Li3 35.29(12) 1_545 3_645 ?
Fe2 Li6 Li3 62.02(14) 7_566 3_645 ?
Li1 Li6 Li3 114.0(2) 7_565 3_645 ?
Fe1 Li6 Li3 175.6(3) 2_565 3_645 ?
Li7 Li6 Li3 126.7(2) 2_565 3_645 ?
F4 Li6 Li3 152.7(3) . 4_465 ?
F8 Li6 Li3 24.55(15) 8_646 4_465 ?
O2 Li6 Li3 72.30(18) 2_565 4_465 ?
F5 Li6 Li3 101.0(2) 2_565 4_465 ?
O1 Li6 Li3 103.6(2) 7_566 4_465 ?
F7 Li6 Li3 80.3(2) 1_545 4_465 ?
Fe2 Li6 Li3 61.58(14) 7_566 4_465 ?
Li1 Li6 Li3 118.9(2) 7_565 4_465 ?
Fe1 Li6 Li3 89.56(16) 2_565 4_465 ?
Li7 Li6 Li3 67.4(2) 2_565 4_465 ?
Li3 Li6 Li3 90.13(19) 3_645 4_465 ?
F3 Li7 F7 84.2(2) 3_655 7_576 ?
F3 Li7 F5 171.2(5) 3_655 . ?
F7 Li7 F5 103.3(3) 7_576 . ?
F3 Li7 F1 99.1(2) 3_655 . ?
F7 Li7 F1 155.6(6) 7_576 . ?
F5 Li7 F1 76.1(2) . . ?
F3 Li7 F2 74.3(3) 3_655 7_566 ?
F7 Li7 F2 127.4(4) 7_576 7_566 ?
F5 Li7 F2 97.3(3) . 7_566 ?
F1 Li7 F2 76.2(2) . 7_566 ?
F3 Li7 F4 105.4(4) 3_655 7_566 ?
F7 Li7 F4 75.3(2) 7_576 7_566 ?
F5 Li7 F4 72.5(2) . 7_566 ?
F1 Li7 F4 126.0(4) . 7_566 ?
F2 Li7 F4 65.7(3) 7_566 7_566 ?
F3 Li7 Li3 43.86(15) 3_655 5_676 ?
F7 Li7 Li3 40.82(15) 7_576 5_676 ?
F5 Li7 Li3 142.6(3) . 5_676 ?
F1 Li7 Li3 140.2(3) . 5_676 ?
F2 Li7 Li3 100.3(3) 7_566 5_676 ?
F4 Li7 Li3 85.2(2) 7_566 5_676 ?
F3 Li7 Fe1 136.5(3) 3_655 . ?
F7 Li7 Fe1 136.8(3) 7_576 . ?
F5 Li7 Fe1 38.10(12) . . ?
F1 Li7 Fe1 38.04(11) . . ?
F2 Li7 Fe1 85.3(2) 7_566 . ?
F4 Li7 Fe1 100.1(2) 7_566 . ?
Li3 Li7 Fe1 173.6(4) 5_676 . ?
F3 Li7 Li2 82.9(2) 3_655 3_655 ?
F7 Li7 Li2 160.3(4) 7_576 3_655 ?
F5 Li7 Li2 88.7(2) . 3_655 ?
F1 Li7 Li2 42.32(14) . 3_655 ?
F2 Li7 Li2 33.97(9) 7_566 3_655 ?
F4 Li7 Li2 93.9(3) 7_566 3_655 ?
Li3 Li7 Li2 123.2(2) 5_676 3_655 ?
Fe1 Li7 Li2 60.50(12) . 3_655 ?
F3 Li7 Li5 36.2(2) 3_655 1_556 ?
F7 Li7 Li5 104.6(3) 7_576 1_556 ?
F5 Li7 Li5 135.6(4) . 1_556 ?
F1 Li7 Li5 91.3(2) . 1_556 ?
F2 Li7 Li5 38.43(17) 7_566 1_556 ?
F4 Li7 Li5 82.0(3) 7_566 1_556 ?
Li3 Li7 Li5 66.8(2) 5_676 1_556 ?
Fe1 Li7 Li5 117.4(2) . 1_556 ?
Li2 Li7 Li5 56.94(16) 3_655 1_556 ?
F3 Li7 Li1 142.4(4) 3_655 . ?
F7 Li7 Li1 88.1(2) 7_576 . ?
F5 Li7 Li1 35.35(19) . . ?
F1 Li7 Li1 102.9(3) . . ?
F2 Li7 Li1 81.7(3) 7_566 . ?
F4 Li7 Li1 37.26(16) 7_566 . ?
Li3 Li7 Li1 116.0(3) 5_676 . ?
Fe1 Li7 Li1 67.63(17) . . ?
Li2 Li7 Li1 93.1(2) 3_655 . ?
Li5 Li7 Li1 112.7(3) 1_556 . ?
F3 Li7 Li6 147.4(5) 3_655 2_565 ?
F7 Li7 Li6 79.6(2) 7_576 2_565 ?
F5 Li7 Li6 40.48(17) . 2_565 ?
F1 Li7 Li6 85.2(3) . 2_565 ?
F2 Li7 Li6 137.4(3) 7_566 2_565 ?
F4 Li7 Li6 97.6(2) 7_566 2_565 ?
Li3 Li7 Li6 117.7(3) 5_676 2_565 ?
Fe1 Li7 Li6 58.15(16) . 2_565 ?
Li2 Li7 Li6 118.6(2) 3_655 2_565 ?
Li5 Li7 Li6 175.4(3) 1_556 2_565 ?
Li1 Li7 Li6 65.34(19) . 2_565 ?

_refine_diff_density_max         0.462
_refine_diff_density_min         -0.400
_refine_diff_density_rms         0.107

